| ||Format||Pages||Price|| |
|8||$46.00||  ADD TO CART|
|Hardcopy (shipping and handling)||8||$46.00||  ADD TO CART|
|Standard + Redline PDF Bundle||16||$55.20||  ADD TO CART|
Significance and Use
4.1 This test method assigns an empirical value to the relative amount, fineness, and character of clay-like material that may be generated in an aggregate when subjected to mechanical degradation.
4.2 The procedure has been used in limited geographical areas of the United States, and the results have been correlated with aggregate performance in various construction applications, including: aggregate base, permeable material for backfill, fine concrete aggregate, and riprap for rock slope protection.,
4.3 A minimum durability index is permitted to be specified to prohibit the use of an aggregate in various construction applications that is prone to degradation, resulting in generation of clay-like fines.
4.4 This test method provides a rapid test for evaluation of the quality of a new aggregate source. Research has indicated it may also be suitable for use instead of the sodium sulfate soundness test for evaluating the durability characteristics of fine aggregate for use in portland cement concrete, thereby reducing the need for time-consuming and expensive soundness tests.
4.5 Although the application of this method has been limited to aggregates for specific construction uses, the possibility exists for expanding the application of this method to control the quality of aggregates used in other areas of construction, such as aggregates for use in bituminous paving mixtures, coarse aggregate for use in portland cement concrete, and aggregate for use as railroad ballast.
Note 1: The text of this test method references notes and footnotes which provide explanatory material. These notes and footnotes (excluding those in tables and figures) shall not be considered as requirements of the test method.
Note 2: The quality of the results produced by this standard are dependent on the competence of the personnel performing the procedure and the capability, calibration, and maintenance of the equipment used. Agencies that meet the criteria of Specification are generally considered capable of competent and objective testing, sampling, inspection, etc. Users of this standard are cautioned that compliance with Specification alone does not completely ensure reliable results. Reliable results depend on many factors; following the suggestions of Specification or some similar acceptable guideline provides a means of evaluating and controlling some of those factors.
1.1 This test method covers the determination of a durability index of an aggregate. The calculated durability index is a value indicating the relative resistance of an aggregate to production of detrimental clay-like fines when subjected to the prescribed mechanical methods of degradation.
1.2 Units—The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in nonconformance with the standard.
1.2.1 Measurements of volume and mass are only given in SI units because they are the only units typically used in practice when performing this test method.
1.2.2 Measurements in Section , Section , , , and Table 1 are only given in inch-pound units because the equipment used in these sections is only manufactured using the inch-pound system.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.4 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C127 Test Method for Relative Density (Specific Gravity) and Absorption of Coarse Aggregate
C136/C136M Test Method for Sieve Analysis of Fine and Coarse Aggregates
C702/C702M Practice for Reducing Samples of Aggregate to Testing Size
D75/D75M Practice for Sampling Aggregates
D2419 Test Method for Sand Equivalent Value of Soils and Fine Aggregate
D3666 Specification for Minimum Requirements for Agencies Testing and Inspecting Road and Paving Materials
D4753 Guide for Evaluating, Selecting, and Specifying Balances and Standard Masses for Use in Soil, Rock, and Construction Materials Testing
E11 Specification for Woven Wire Test Sieve Cloth and Test Sieves
ICS Number Code 93.080.10 (Road construction); 93.080.20 (Road construction materials)
UNSPSC Code 30111800(Aggregates)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D3744 / D3744M-18, Standard Test Method for Aggregate Durability Index, ASTM International, West Conshohocken, PA, 2018, www.astm.orgBack to Top